Effect of Metal Complexing on Mn–Fe/TS-1 Catalysts for Selective Catalytic Reduction of NO with NH3

TS-1 zeolite with desirable pore structure, an abundance of acidic sites, and good thermal stability promising as a support for the selective catalytic reduction of NO with NH3 (NH3-SCR). Herein, a series of Mn–Fe/TS-1 catalysts have been synthesized, adopting tetraethylenepentamine (TEPA) as a metal complexing agent using the one-pot hydrothermal method. The introduced TEPA can not only increase the loading of active components but also prompts the formation of a hierarchical structure through decreasing the size of TS-1 nanocrystals to produce intercrystalline mesopores during the hydrothermal crystallization process. The optimized Mn–Fe/TS-1(R-2) catalyst shows remarkable NH3-SCR performance. Moreover, it exhibits excellent resistance to H2O and SO2 at low temperatures. The characterization results indicate that Mn–Fe/TS-1(R-2) possesses abundant surface Mn4+ and Fe2+ and chemisorbed oxygen, strong reducibility, and a high Brønsted acid amount. For comparison, Mn–Fe/TiO2 displays a narrower active temperature window due to its poor thermostability.


Introduction
Nitrogen oxides (NO x ) are associated with a host of environmental issues, such as acid rain, haze, and photochemical smog, which severely endanger public health [1,2]. Selective catalytic reduction of nitrogen oxides with ammonia (NH 3 -SCR) is a crucial method to effectively control NO x emission [3,4]. Presently, the commercial V 2 O 5 -WO 3 /TiO 2 (VWTi) catalyst is employed extensively for controlling NO x emissions. However, there are still many problems in the practical application of the VWTi catalyst, such as narrow temperature windows, poor high-temperature stability, the poisonousness of V 2 O 5 , and so on [5,6]. Accordingly, numerous studies have been devoted to exploiting vanadium-free NH 3 -SCR catalysts in recent years.
Among the frequently adopted V-free metal oxide catalysts, Mn-based catalysts have been proven to be remarkable low-temperature denitrification catalysts due to polyvalent oxidation and high redox capabilities [7,8]. However, the practical application of singlemetal MnO x catalysts is restricted due to their narrow operating temperature window, and poor H 2 O/SO 2 resistance [9,10]. Therefore, other transition metals/rare earth metal oxides serve as active components to perfect the Mn-based catalysts and improve the denitrification performance [11,12]. In recent years, Mn-Fe composite catalysts have gained extensive attention for their superior SCR activity and tolerance to SO 2 /H 2 O at low temperatures [13][14][15]. Li et al. [16] reported that Fe 2 O 3 -MnO 2 /TiO 2 catalyst synthesized through a conventional impregnation method displayed excellent low-temperature activity in the wide temperature range of 100−325 • C and superior sulfur poisoning resistance. Additionally, Chen et al. [17] investigated La-modified TiO 2 as the support of Fe-Mn/TiO 2 (x La) 2 of 13 catalyst for NH 3 -SCR at low temperatures, revealing that La-modified Fe-Mn/TiO 2 (x La) catalyst enhanced SO 2 resistance through an increase in Brønsted acid sites and accelerating the electron transfer between La and active components to restrain the adsorption and oxidation of SO 2 on the catalyst. Nevertheless, TiO 2 as a support in NH 3 -SCR possesses poor thermal stability and is still unsatisfactory for practical application [18].
It has been reported that silicon atoms replacing a small number of titanium atoms to form TS-1 zeolite with MFI structure can improve thermal stability and surface acidity [19]. Wang et al. [20] obtained MnO x -FeO x /TS-1 via a wet impregnation method, and the catalyst with the TS-1 support displayed superior denitration ability and H 2 O resistance due to the enhanced surface acidity and redox ability. Considering that NH 3 -SCR performance could be influenced by controlling the pore structure of the TS-1 support, a novel Fe−Mn/TS-1 catalyst with a micro-mesoporous structure was prepared using a one-pot hydrothermal synthesis method. The Fe−Mn/TS-1 catalyst showed excellent catalytic activity and H 2 O/SO 2 resistance in a low-temperature SCR reaction. The influence of the additional quantity of metal complexing agent TEPA on NO x conversion has been investigated, and the SO 2 and H 2 O resistance has also been explored.  23.8, and 24.3 • are indexed to the MFI structure, meaning the addition of TEPA into the synthesis gel does not transform the phase texture of the TS-1 under hydrothermal synthesis or calcination. However, the peak intensities have been affected. He et al. [21] reported that the diffraction peak intensity increases with an increase in crystallinity. Mn-Fe/TS-1(R-0.5), Mn-Fe/TS-1(R-1), and Mn-Fe/TS-1(R-2) display lower crystallinity than Mn-Fe/TS-1(R-0), ascribed to the existence of small crystallites [22]. Furthermore, the crystalline phases of Mn and Fe species are not detected in Mn-Fe/TS-1(R-x) catalysts, indicating that the particle size of Mn and Fe species is too small to be detected; the Mn and Fe species are amorphous [23].

XRD Patterns
temperatures [13][14][15]. Li et al. [16] reported that Fe2O3-MnO2/TiO2 catalyst synthesized through a conventional impregnation method displayed excellent low-temperature activity in the wide temperature range of 100−325 °C and superior sulfur poisoning resistance. Additionally, Chen et al. [17] investigated La-modified TiO2 as the support of Fe-Mn/TiO2(x La) catalyst for NH3-SCR at low temperatures, revealing that La-modified Fe-Mn/TiO2(x La) catalyst enhanced SO2 resistance through an increase in Brønsted acid sites and accelerating the electron transfer between La and active components to restrain the adsorption and oxidation of SO2 on the catalyst. Nevertheless, TiO2 as a support in NH3-SCR possesses poor thermal stability and is still unsatisfactory for practical application [18].
It has been reported that silicon atoms replacing a small number of titanium atoms to form TS-1 zeolite with MFI structure can improve thermal stability and surface acidity [19]. Wang et al. [20] obtained MnOx-FeOx/TS-1 via a wet impregnation method, and the catalyst with the TS-1 support displayed superior denitration ability and H2O resistance due to the enhanced surface acidity and redox ability. Considering that NH3-SCR performance could be influenced by controlling the pore structure of the TS-1 support, a novel Fe−Mn/TS-1 catalyst with a micro-mesoporous structure was prepared using a onepot hydrothermal synthesis method. The Fe−Mn/TS-1 catalyst showed excellent catalytic activity and H2O/SO2 resistance in a low-temperature SCR reaction. The influence of the additional quantity of metal complexing agent TEPA on NOx conversion has been investigated, and the SO2 and H2O resistance has also been explored. Figure 1 displays the XRD patterns of Mn-Fe/TS-1(R-0), Mn-Fe/TS-1(R-0.5), Mn-Fe/TS-1(R-1), and Mn-Fe/TS-1(R-2). The diffraction peaks at 7.9, 8.8, 23.1, 23.8, and 24.3° are indexed to the MFI structure, meaning the addition of TEPA into the synthesis gel does not transform the phase texture of the TS-1 under hydrothermal synthesis or calcination. However, the peak intensities have been affected. He et al. [21] reported that the diffraction peak intensity increases with an increase in crystallinity. Mn-Fe/TS-1(R-0.5), Mn-Fe/TS-1(R-1), and Mn-Fe/TS-1(R-2) display lower crystallinity than Mn-Fe/TS-1(R-0), ascribed to the existence of small crystallites [22]. Furthermore, the crystalline phases of Mn and Fe species are not detected in Mn-Fe/TS-1(R-x) catalysts, indicating that the particle size of Mn and Fe species is too small to be detected; the Mn and Fe species are amorphous [23].

FT−IR Spectroscopy
The FT−IR spectra of Mn-Fe/TS-1(R-0), Mn-Fe/TS-1(R-0.5), Mn-Fe/TS-1(R-1), and Mn-Fe/TS-1(R-2) are shown in Figure 2. All samples display infrared peaks at 1100, 960, 800, 550, and 450 cm −1 . The band at 550 cm −1 is assigned to the vibration of the double five-membered ring unit and demonstrates the formation of MFI structure. The bands at 800 and 1100 cm −1 are attributed to the symmetrical and antisymmetrical stretching vibrations of Si-O-Si bonds, respectively. The band at 960 cm −1 has been used as evidence of the isomorphous substitution of Ti in the TS-1 framework [24]. Moreover, the intensity ratio of the bands at 550 and 450 cm −1 (I 550 /I 450 ) has been often used to evaluate the crystallinity of MFI zeolite, which is termed as the FTIR crystallinity [25,26]. The I 550 /I 450 ratios for the Mn-Fe/TS-1(R-0), Mn-Fe/TS-1(R-0.5), Mn-Fe/TS-1(R-1), and Mn-Fe/TS-1(R-2) are 0.66, 0.52, 0.59, and 0.54, respectively, demonstrating that Mn-Fe/TS-1 synthesized using TEPA as a metal complexing agent has low crystallinity, which is in good agreement with the XRD results.

N2 Adsorption-Desorption
The N2 adsorption-desorption isotherms of Mn-Fe/TS-1(R-0), Mn-Fe/TS-1(R-0.5), Mn-Fe/TS-1(R-1), and Mn-Fe/TS-1(R-2) are presented in Figure 3 and the textural properties of the catalysts are presented in Table 1. All of the Mn-Fe/TS-1(R-x) samples displayed standard type I isotherms in the relative pressures of p/p0 < 0.01, indicating that the samples have microporous structure. Meanwhile, an uptake in the relative pressures of 0.60 < p/p0 < 1.0 can be observed due to the intercrystalline mesopores, which is typical of the nanocrystal structure of TS-1 [27]. The hierarchical structure of the samples is conducive to enhancing the diffusion of reactant and product molecules [28]. Moreover, the Mn-Fe/TS-1(R-2) catalyst displays a higher content of active metal components (3.9 wt% Mn and 4.9 wt% Fe) than Mn-Fe/TS-1(R-0, 0.5 wt% Mn and 2 wt% Fe), which demonstrates that the suitable addition of TEPA is conducive to increasing a number of active components. Significantly, high levels of Mn and Fe in Mn-Fe/TiO2 prepared by the impregnation method can be observed, which promote most of the active ingredient loaded on the support and reduce the level of the active ingredient dispersion.

N 2 Adsorption-Desorption
The N 2 adsorption-desorption isotherms of Mn-Fe/TS-1(R-0), Mn-Fe/TS-1(R-0.5), Mn-Fe/TS-1(R-1), and Mn-Fe/TS-1(R-2) are presented in Figure 3 and the textural properties of the catalysts are presented in Table 1. All of the Mn-Fe/TS-1(R-x) samples displayed standard type I isotherms in the relative pressures of p/p 0 < 0.01, indicating that the samples have microporous structure. Meanwhile, an uptake in the relative pressures of 0.60 < p/p 0 < 1.0 can be observed due to the intercrystalline mesopores, which is typical of the nanocrystal structure of TS-1 [27]. The hierarchical structure of the samples is conducive to enhancing the diffusion of reactant and product molecules [28]. Moreover, the Mn-Fe/TS-1(R-2) catalyst displays a higher content of active metal components (3.9 wt% Mn and 4.9 wt% Fe) than Mn-Fe/TS-1(R-0, 0.5 wt% Mn and 2 wt% Fe), which demonstrates that the suitable addition of TEPA is conducive to increasing a number of active components. Significantly, high levels of Mn and Fe in Mn-Fe/TiO 2 prepared by the impregnation method can be observed, which promote most of the active ingredient loaded on the support and reduce the level of the active ingredient dispersion.

SEM Images and EDS Analysis
The morphology and particle size of Mn-Fe/TS-1(R-x) were characterized by SEM, as shown in Figure 4. The calcined Mn-Fe/TS-1(R-x) shows granular morphology with a rough surface. The particle size of Mn-Fe/TS-1(R-0) is 400-700 nm ( Figure 4a). Interestingly, with the introduction of a small amount of TEPA for Mn-Fe/TS-1(R-0.5), the crystal size reduces to 200-350 nm ( Figure 4b). However, upon further increasing the TEPA amount, the crystal size significantly increases again from 270-400 nm to 300-450 nm for Mn-Fe/TS-1(R-1) ( Figure 4c) and Mn-Fe/TS-1(R-2) (Figure 4d), respectively. The results show that the addition of TEPA does not restrain the generation of TS-1, but influences the crystallinity of TS-1 to a certain extent in accordance with the XRD results. The EDX mapping of the Mn-Fe/TS-1(R-2) (Figure 4e) indicates that excluding Si and Ti, which constitute the framework of TS-1, Mn and Fe are also detected in the crystallite. Therefore, Mn and Fe species may be incorporated into the structure of the skeleton or cationic sites and may be highly dispersed over the catalyst [29].

SEM Images and EDS Analysis
The morphology and particle size of Mn-Fe/TS-1(R-x) were characterized by SEM, as shown in Figure 4. The calcined Mn-Fe/TS-1(R-x) shows granular morphology with a rough surface. The particle size of Mn-Fe/TS-1(R-0) is 400-700 nm (Figure 4a). Interestingly, with the introduction of a small amount of TEPA for Mn-Fe/TS-1(R-0.5), the crystal size reduces to 200-350 nm (Figure 4b). However, upon further increasing the TEPA amount, the crystal size significantly increases again from 270-400 nm to 300-450 nm for Mn-Fe/TS-1(R-1) (Figure 4c) and Mn-Fe/TS-1(R-2) (Figure 4d), respectively. The results show that the addition of TEPA does not restrain the generation of TS-1, but influences the crystallinity of TS-1 to a certain extent in accordance with the XRD results. The EDX mapping of the Mn-Fe/TS-1(R-2) (Figure 4e) indicates that excluding Si and Ti, which constitute the framework of TS-1, Mn and Fe are also detected in the crystallite. Therefore, Mn and Fe species may be incorporated into the structure of the skeleton or cationic sites and may be highly dispersed over the catalyst [29].

XPS Analysis
The surface composition and chemical state of Mn, Fe, O, and Ti of the diffe catalysts were characterized by XPS ( Figure 5). As shown in Figure 5a, the Mn 2p spectra exhibit two main peaks, associated with Mn 2p1/2 (~653 eV) and Mn 2p3/2 (~642

XPS Analysis
The surface composition and chemical state of Mn, Fe, O, and Ti of the different catalysts were characterized by XPS ( Figure 5). As shown in Figure 5a, the Mn 2p XPS spectra exhibit two main peaks, associated with Mn 2p 1/2 (~653 eV) and Mn 2p 3/2 (~642 eV). The Mn 2p 3/2 spectra of the catalysts are de-convoluted into oxidation states of Mn 2+ , Mn 3+ , and Mn 4+ which are observed at 641.3, 642.5, and 644.2 eV, respectively. Moreover, the relative ratios of Mn 4+ /Mn suf for all the catalysts were calculated and the results are listed in Table 2. The Mn 4+ /Mn suf values of Mn-Fe/TS-1(R-0.5) and Mn-Fe/TS-1(R-2) are significantly higher than that of others. Combined with the denitration results of the catalysts, the greater Mn 4+ can accelerate the transformation of NO to NO 2 and further promote the occurrence of a "fast SCR" reaction [30].  The O 1 s spectra of the catalysts are deconvoluted into three peaks as shown in Figure 5c, corresponding to the lattice oxygen (represented by Oβ) at around 530 eV, surface chemisorbed oxygen (represented by Oα) at around 531 eV, and -OH (represented by Oα') at around 532.8 eV. The surface chemisorbed oxygen is an extremely active oxygen species that plays a key role in oxidation reactions attributed to more rapid migration than  The Fe 2p XPS spectra are shown in Figure 5b, and display two main peaks of Fe 2p 1/2 and Fe 2p 3/2 . The Fe 2p 3/2 peak is deconvoluted into different states of Fe consisting of Fe 2+ and Fe 3+ species, which appear at 710 eV and 711 eV [31], respectively. The relative ratio of Fe 2+ /Fe suf is increased from 8.71% (Mn-Fe/TS-1(R-0)) to 15.8% (Mn-Fe/TS-1(R-2)) with the increased addition of TEPA. Compared with Mn-Fe/TiO 2 catalyst prepared by the wet impregnation method, the relative ratio of Fe 2+ /Fe suf over the Mn-Fe/TS-1(R-2) catalyst is higher. Therefore, the Mn-Fe/TS-1(R-2) catalyst has more active sites to accelerate the SCR reaction. The atomic concentration of the Mn-Fe/TS-1(R-2) (0.21 % Mn, 3.43 % Fe, Table 2) catalyst is lower than that of Mn-Fe/TS-1(R-0, 0.5, 1), which demonstrates that the majority of the active metal component on the surface is in the form of Mn 4+ and Fe 2+ .
The O 1 s spectra of the catalysts are deconvoluted into three peaks as shown in Figure 5c, corresponding to the lattice oxygen (represented by O β ) at around 530 eV, surface chemisorbed oxygen (represented by O α ) at around 531 eV, and -OH (represented by O α' ) at around 532.8 eV. The surface chemisorbed oxygen is an extremely active oxygen species that plays a key role in oxidation reactions attributed to more rapid migration than the other oxygen species. Therefore, the high O α /O suf atomic ratio is conducive to accelerating the transformation of NO to NO 2 to improve the NH 3 -SCR reaction performance. The relative ratio of O α /O suf decreases in the following order: Mn-Fe/TS-1(R-0) > Mn-Fe/TS-1(R-2) > Mn-Fe/TS-1(R-1) > Mn-Fe/TiO 2 > Mn-Fe/TS-1(R-0.5). Furthermore, the O α' peak intensity of Mn-Fe/TS-1(R-x) catalysts is stronger than that of Mn-Fe/TiO 2 . The results illustrate that Mn-Fe/TS-1(R-x) catalysts possess more -OH than the Mn-Fe/TiO 2 catalyst, which is mainly derived from the Si-OH and Ti-OH of the TS-1 support [31].
The Ti 2p XPS spectra of all catalysts show two main peaks as shown in Figure 5d, associated with Ti 2p 1/2 (~464.3 eV) and Ti 2p 3/2 (~458.3 eV). The results indicate that Ti 4+ is the main valence state of all catalysts [32]. The sectional Ti atoms in the TiO 2 support are replaced by Si, and the binding energy of the Mn-Fe/TS-1(R-x) catalyst shifts to a high value, indicating that the introduction of Si affects the chemical environment of Ti 4+ in the catalyst.

H 2 -TPR
The reducibility of catalysts closely correlates with the catalytic performance of the NH 3 -SCR reaction. Hence, H 2 -TPR experiments were carried out to characterize the reducibility of the catalysts and the result are displayed in Figure 6. The H 2 consumption peaks are observed from 100 to 800 • C in all catalysts, which are related to the reduction process of MnO x and FeO x . Mn-Fe/TiO 2 catalyst exhibits four obvious reduction peaks. The first peak at low temperatures (~281 • C) is assigned to the reduction of MnO 2 to Mn 2 O 3 . The second reduction peak at around 363 • C is attributed to the reduction of Mn 2  → FeO). The reduction peak located at 530-610 • C is associated with the reduction of Mn 3 O 4 , while the high-temperature reduction peaks (590-690 • C) are related to the reduction of FeO [34]. When Si species were introduced into the TiO 2 support, H 2 consumption of the Mn-Fe/TS-1(R-x) catalysts was larger than that of the Mn-Fe/TiO 2 catalyst (Table 3). It is worth noting that the Mn-Fe/TS-1(R-2) catalyst displays higher H 2 consumption than the others, indicating that it possesses enhanced redox properties. The improved reducibility is beneficial to promote the NH 3 -SCR reaction. 610 °C is associated with the reduction of Mn3O4, while the high-temperature reduction peaks (590-690 °C) are related to the reduction of FeO [34]. When Si species were introduced into the TiO2 support, H2 consumption of the Mn-Fe/TS-1(R-x) catalysts was larger than that of the Mn-Fe/TiO2 catalyst (Table 3). It is worth noting that the Mn-Fe/TS-1(R-2) catalyst displays higher H2 consumption than the others, indicating that it possesses enhanced redox properties. The improved reducibility is beneficial to promote the NH3-SCR reaction.

NH 3 -TPD
The catalyst surface acidity is a very crucial influencing factor in low-temperature SCR reactions, and the acidity of the catalysts was determined by NH 3 -TPD. According to previous studies [35,36], the coordinated NH 3 molecules bound to Lewis acid sites is more thermally stable than the NH 4 + ions fixed on Brønsted acid sites, so it could be conjectured that the desorption peak at low temperatures is assigned to NH 4 + ions bound to the Brønsted acid sites, while the desorption peak at high temperatures is associated with NH 3 molecules originating from the Lewis acid sites. Moreover, the area of desorption peaks is directly proportional to the acid amount and the peak position is correlated with the acid strength. As shown in Figure 7, three ammonia desorption peaks are discovered in the Mn-Fe/TiO 2 catalyst; the desorption peak at low temperatures (~193 • C) is generated by the physical adsorption of NH 3 , the desorption peak at 200-300 • C is attributed to the Brønsted acid site, and the desorption peak at high temperatures (~518 • C) is attributed to the Lewis acid site [34]. It is worth noting that Mn-Fe/TS-1(R-x) catalysts display two desorption peaks. The desorption peak at low temperatures (<200 • C) is attributed to the physical adsorption of NH 3 , and the peak at high temperatures (200-400 • C) is ascribed to the Brønsted acid site [37]. Previous research indicates that the Brønsted acid site could reserve NH 3 and enhance SCR reaction activity [38,39]. The amounts of different acid sites are calculated from the NH 3 -TPD results. As listed in Table 4, the Brønsted acid amount of Mn-Fe/TS-1(R-2) (centered at around 267 • C) is higher than those of others catalysts, which is conducive to improving the SCR reaction, indicating that the substitution of Si species into the TiO 2 support can enhance the surface acidity of the catalyst and the adsorption and activation of ammonia, thus improving the catalytic activity in low-temperature SCR reactions. The acidic properties of the catalysts were also analyzed by pyridine IR spectroscopy ( Figure S1 in Supplementary Materials). IR bands at~1445 and 1540 cm −1 observed in the spectra can be attributed to pyridine adsorption related to Lewis and Brønsted acid sites, respectively. The Mn-Fe/TS-1(R-2) exhibits a higher peak area of Brønsted acid sites than the other samples, indicating that the amount of Brønsted acid sites on Mn-Fe/TS-1(R-2) catalyst was significantly increased compared with the other catalysts. This is consistent with the NH 3 -TPD result.  To study the influence of TS-1 support on NH3-SCR reactions, the NOx conversion over the Mn-Fe/TiO2 catalyst prepared by the wet impregnation method was also evaluated. Mn-Fe/TiO2 and Mn-Fe/TS-1(R-2) show higher NOx conversion than other catalysts at low temperatures (<200 °C). However, the NOx conversion of Mn-Fe/TiO2 decreases due to the generation of N2O and NO2 byproducts at high temperatures (when the reaction temperature increases above 250 °C) [14]. Furthermore, TiO2 support undergoes phase transition at high temperatures (>550 °C), leading to narrow temperature windows for SCR reactions. In contrast, the NH3-SCR activity of Mn-Fe/TS-1(R-x) catalysts is maintained well and only a slight decline in NOx conversion is observed at high temperatures (>250 °C) due to high thermal stability and the enhanced acidity of TS-1 support. It is worth noting that the Mn-Fe/TS-1(R-2) catalyst exhibits remarkably improved catalytic activity with more than 80% NOx conversion in a wide temperature range of 170-325 °C. Furthermore, Mn-Fe/TS-1 catalysts synthesized using the wet impregnation method were reported by Wang et al. [20], demonstrating that the optimized Mn3-Fe2/TS-1-30 can maintain steady NOx conversion efficiencies above  Table 4. Acid properties of the samples obtained from NH 3 -TPD.

Samples
Temperature ( • C)/NH 3 Adsorption Amount (mL·g −1 , STP) To study the influence of TS-1 support on NH 3 -SCR reactions, the NO x conversion over the Mn-Fe/TiO 2 catalyst prepared by the wet impregnation method was also evaluated. Mn-Fe/TiO 2 and Mn-Fe/TS-1(R-2) show higher NO x conversion than other catalysts at low temperatures (<200 • C). However, the NO x conversion of Mn-Fe/TiO 2 decreases due to the generation of N 2 O and NO 2 byproducts at high temperatures (when the reaction temperature increases above 250 • C) [14]. Furthermore, TiO 2 support undergoes phase transition at high temperatures (>550 • C), leading to narrow temperature windows for SCR reactions. In contrast, the NH 3 -SCR activity of Mn-Fe/TS-1(R-x) catalysts is maintained well and only a slight decline in NO x conversion is observed at high temperatures (>250 • C) due to high thermal stability and the enhanced acidity of TS-1 support. It is worth noting that the Mn-Fe/TS-1(R-2) catalyst exhibits remarkably improved catalytic activity with more than 80% NO x conversion in a wide temperature range of 170-325 • C. Furthermore, Mn-Fe/TS-1 catalysts synthesized using the wet impregnation method were reported by Wang et al. [20], demonstrating that the optimized Mn 3 -Fe 2 /TS-1-30 can maintain steady NO x conversion efficiencies above 80% in the temperature range of 110-230 • C with a space velocity of 18,000 h −1 . Meanwhile, Mn-Fe/TS-1(R-2) prepared by the one-pot hydrothermal method displays wider temperature ranges with high GHSV than the Mn 3 -Fe 2 /TS-1-30 catalyst. The resistance to H2O and SO2 poisoning was further evaluated over the Mn-Fe/TS-1(R-x) and Mn-Fe/TiO2 catalysts, and the results are shown in Figure 8b. Previous research results show that H2O and SO2 combine with NH3 to produce NH4HSO4 with the coexistence of H2O and SO2 [28,40], and the NH4HSO4 cannot decompose below 300 °C [41]. As can be seen in Figure 8b, the NOx conversion of Mn-Fe/TS-1(R-x) markedly decreases with the introduction of H2O and SO2 at low temperatures (≤300 °C). Conversely, the inhibition effect on the NH3-SCR activity of Mn-Fe/TiO2 is less than that of Mn-Fe/TS-1(R-x) in the presence of H2O and SO2. More than 80% NOx conversion is achieved over the Mn-Fe/TiO2 catalyst at 150-300 °C, which may be ascribed to the regeneration of the acid site from NH4HSO4 on the catalyst surface. When the temperature reaches 350 °C, the NOx conversion of the Mn-Fe/TiO2 catalyst decreases to 65% due to the decomposition of NH4HSO4 covered on the surface at high temperatures (>300 °C). It is important to note that the NOx conversion of the Mn-Fe/TS-1(R-2) catalyst reaches a value above 80% at temperatures above 200 °C, indicating that the catalytic activity is less affected by the introduction of H2O and SO2. The enhanced H2O and SO2 tolerance obtained with Mn-Fe/TS-1(R-2) may be due to the addition of a suitable amount of complexing agent TEPA, which facilitates more active component loading of the TS-1 support and a micro-mesoporous structure beneficial for the adsorption and diffusion of the reactants and products. Based on the above results, titanosilicate TS-1 support with desirable pore structure and enriched isolated framework Ti species can enhance SCR activity. It is important to point out that SSZ-13 has been commonly used in NH3-SCR reactions due to its unique pore configuration and acidity properties. However, tetracoordinated titanium-incorporated SSZ-13 zeolites show stronger Brønsted acidity and hydrothermal stability than SSZ-13 [42], indicating them as a promising SCR catalyst in the future.

Catalyst Preparation
The precursors of the silicon source and titanium source were tetraethylorthosilicate (99%, TEOS, innochem) and tetrabutyl orthotitanate (98%, TBOT, Aladdin), respectively. Tetraethylenepentamine (TEPA, Aladdin) was used as the complexing agent, and tetrapropyl ammonium hydroxide (25%, TPAOH, innochem) was employed as a  [28,40], and the NH 4 HSO 4 cannot decompose below 300 • C [41]. As can be seen in Figure 8b, the NO x conversion of Mn-Fe/TS-1(R-x) markedly decreases with the introduction of H 2 O and SO 2 at low temperatures (≤300 • C). Conversely, the inhibition effect on the NH 3 -SCR activity of Mn-Fe/TiO 2 is less than that of Mn-Fe/TS-1(R-x) in the presence of H 2 O and SO 2 . More than 80% NO x conversion is achieved over the Mn-Fe/TiO 2 catalyst at 150-300 • C, which may be ascribed to the regeneration of the acid site from NH 4 HSO 4 on the catalyst surface. When the temperature reaches 350 • C, the NO x conversion of the Mn-Fe/TiO 2 catalyst decreases to 65% due to the decomposition of NH 4 HSO 4 covered on the surface at high temperatures (>300 • C). It is important to note that the NO x conversion of the Mn-Fe/TS-1(R-2) catalyst reaches a value above 80% at temperatures above 200 • C, indicating that the catalytic activity is less affected by the introduction of H 2 O and SO 2 . The enhanced H 2 O and SO 2 tolerance obtained with Mn-Fe/TS-1(R-2) may be due to the addition of a suitable amount of complexing agent TEPA, which facilitates more active component loading of the TS-1 support and a micro-mesoporous structure beneficial for the adsorption and diffusion of the reactants and products. Based on the above results, titanosilicate TS-1 support with desirable pore structure and enriched isolated framework Ti species can enhance SCR activity. It is important to point out that SSZ-13 has been commonly used in NH 3 -SCR reactions due to its unique pore configuration and acidity properties. However, tetra-coordinated titanium-incorporated SSZ-13 zeolites show stronger Brønsted acidity and hydrothermal stability than SSZ-13 [42], indicating them as a promising SCR catalyst in the future.
The crystal seed of TS-1 was prepared with a gel composition of 5 SiO 2 :0.1665 TiO 2 :1.5 TPAOH: 150 H 2 O through the following steps: First, 5.63 mL TEOS and 0.28 mL TBOT were mixed well to obtain Solution A. Later, 6.0 mL TPAOH was dissolved in 13.5 mL water to form Solution B. Solution A mixed with Solution B and stirred for 10 h to achieve a uniform gel. The resulting gel was poured into a stainless-steel autoclave for hydrothermal crystallization at 200 • C for 8 h to obtain the crystal seed of TS-1. An amount of 1. For comparison, Mn-Fe/TiO 2 was also synthesized by an impregnation method. A total of 2.04 g Fe(NO 3 ) 3 •9H 2 O and 1.27 g Mn(NO 3 ) 2 •4H 2 O were dissolved in 20 mL water, then 2.1 g TiO 2 (P25) was impregnated into the above solution. The resulting mixture was dried in a water bath at 80 • C to obtain a powder, and calcined under air at 500 • C for 5 h to obtain the Mn-Fe/TiO 2 catalyst.

Catalyst Characterization
A Shimadzu XRD-6000 diffractometer (Shimadzu, Japan) was used to explore the crystal phase using Cu Kα radiation (λ = 0.15418 nm). Fourier transform infrared (FT-IR) spectra of the samples were recorded on a Spectrum 1 spectrometer (PE, Waltham, Mass, USA) using KBr disks. The textural properties of catalysts were investigated using N 2 adsorption-desorption isotherms at 77 K on a Micromeritics ASAP 2460 (Micromeritics, Norcross, Ga, USA). The total surface area (S BET ) was calculated based on the BET formula. The mesopore surface area (S meso ), micropore volume (V micro ), and mesopore volume (V meso ) were determined by the t-plot method. The active metal contents of the catalysts were measured by an Agilent 7500Ce (Agilent, Santa Clara, California, USA) using inductively coupled plasma mass spectrometry (ICP-MS). Morphologies and particle sizes were measured using a scanning electron microscope (Hitachi S-4300) equipped with an energy dispersive spectrometer (EDS) for analyzing the dispersion of metal oxides. Nano Measurer software (China) was used to analyze the size of crystal particles. At least 300 particles per sample were measured for confirming the average particle size. XPS spectroscopy was conducted using a Thermo ESCALAB 250Xi spectrometer (Thermo, Waltham, MA, USA) equipped with a monochromatized Al Ka X-ray source (1486.6 eV). C 1s (binding energy 284.8 eV) served as a reference. Temperature-programmed reduction with hydrogen (H 2 -TPR) was performed on a Micromeritics ChemiSorb 2720 analyzer. A 0.1 g sample was pretreated at 400 • C for 1 h under Ar flow, then cooled down to 40 • C. The sample was heated to 900 • C at a rate of 10 • C/min under a flow (30 mL/min) of 10 vol.% H 2 /Ar. NH 3 temperature-programmed desorption (NH 3 -TPD) was analyzed by the same instruments as those used for H 2 -TPR. The sample (~0.1 g) was preheated in a pure Ar stream (30 mL/min) at 500 • C for 1 h and then cooled to 110 • C. The catalysts were pre-treated in 10 % NH 3 /He for 1 h, followed by Ar purging for 1 h. NH 3 desorption was measured at a ramp of 10 • C min −1 in an Ar flow (30 mL/min) from 110 to 700 • C. The pyridine IR spectra were recorded on a Spectrum 1 spectrometer (PE, USA). The 0.02 g samples were saturated and adsorbed by pyridine at 298 K for 30 min after activization at 773 K for 1 h, and then evacuated at 373 K for 1 h.

Catalytic Test
The NH 3 -SCR activity was measured in a fixed-bed quartz flow tube reactor loaded with a 0.3 g catalyst. The composition of reactant gas was 500 ppm NO, 500 ppm NH 3 , 100 ppm SO 2 (when used), 5 vol % O 2 , 5 vol % H 2 O (when used), and balance N 2 . The total gas flow rate was 100 mL/min and the corresponding gas hourly space velocity (GHSV) was 20,000 mL·g −1 ·h −1 . The concentration data of NO and NO 2 were monitored using an MRU OPTIMA7 flue gas analyzer. The NO x conversion of the catalyst at the steady state was calculated as follows:

Conclusions
A series of Mn-Fe/TS-1(R-x) catalysts have been prepared by utilizing TEPA as a metal complexing agent under hydrothermal conditions for NH 3 -SCR reactions. The effects of the addition amounts of TEPA on the structure and catalytic activity of the Mn-Fe/TS-1 catalysts were investigated, showing that the Mn-Fe/TS-1(R-2) catalyst displayed enhanced NH 3 -SCR activity at low temperatures. Moreover, the introduction of H 2 O/SO 2 had relatively little impact on NO x conversion for the Mn-Fe/TS-1(R-2) catalyst. In contrast, Mn-Fe/TiO 2 showed narrow temperature windows for SCR reactions. The introduction of TEPA could improve the dispersion and loading of the Mn 4+ , Fe 2+ , and surface chemisorbed oxygen. Furthermore, Mn-Fe/TS-1(R-2) displayed enhanced reducibility and high Brønsted acid amounts. Therefore, the addition of the appropriate amount of TEPA effectively optimized the structure of the TS-1 support and enhanced the catalytic activity.  Data Availability Statement: Data is available upon reasonable request from the corresponding authors.

Conflicts of Interest:
The authors declare no conflict of interest.
Sample Availability: Samples of the catalysts are available from the authors.